DETERMINATION OF SPECIFIC GRAVITY OF CEMENT
IS : 2720 – PART – 3
To determine the specific gravity of cement using Le Chatelier Flask or Specific Gravity Bottle.
1) Le Chatelier Flask or Specific Gravity Bottle – 100 ml capacity.
2) Balance capable of weighing accurately upto 0.1 gm.
Weigh a clean and dry Le Chatelier Flask or Specific Gravity Bottle with its stopper (W1). Place a sample of cement upto half of the flask (about 50 gm) and weight with its stopper (W2). Add kerosene (polar liquid) to cement in flask till it is about half full. Mix thoroughly with glass rod to remove entrapped air. Continue stirring and add more kerosene till it is flush with the graduated mark. Dry the outside and weigh (W3). Entrapped air may be removed by vacuum pump, if available. Empty the flask, clean it , refills with clean kerosene, flush with the graduated mark, wipe dry the outside and finally weigh (W4).
Where, W1 = Weight of empty flask ; W2 = Weight of flask + cement ; W3 = Weight of flask + cement + kerosene ; W4 = Weight of flask + kerosene ; 0.79 = Specific gravity of kerosene
Therefore, SPECIFIC GRAVITY OF CEMENT = 3.15 g/cc
For more Information and Videos, Visit LEARNING TECHNOLOGY
LEARNING TECHNOLOGY is a Brand YouTube channel which contains Technical Lectures on “Civil Engineering” from personal field experience. This Channel is maintained by Civil Engineer MUKESH SAH. You can follow him by subscribing channel and HIT the bell for latest updates.
Share, Support, Subscribe, Like !!!
Visit His Official Websites, Facebook Fan Page and Twitter
For Business Enquiry and Help, You can Email him.
►YouTube Channel : www.youtube.com/channel/UCFBgs2fL5-u-29up4_JF8kw
►Email Id : firstname.lastname@example.org
► Facebook Page : www.facebook.com/L-T-1681713582078656
► Twitter : www.twitter.com/LearningTechno3